Web sites and artwork:QPA Sites:QPA - MIA:Extras:MIA website update material:learning text:LT - Mortar Testing Ap#7E2.docPage 1 of 20Final Version
Web sites and artwork:QPA Sites:QPA - MIA:Extras:MIA website update material:learning text:LT - Mortar Testing Ap#7E2.docPage 2 of 20Final Version
BS EN 1015 : Methods of test for mortar for masonry 4
- General requirements 4
- Determination of particle size distribution (by sieve analysis) 5
- Bulk sampling of mortars and preparation of test mortars 6
- Determination of consistence of fresh mortars (by flow table) 6
- Determination of consistence of fresh mortar (by plunger penetration) 7
- Determination of bulk density of fresh mortar 7
- Determination of air content of fresh mortar 8
- Determination of workable life and correction time of fresh mortar 9
- Determination of dry bulk density of hardened mortar 11
- Determination of flexural and compressive strength of hardened mortar 11
- Determination of adhesive strength of hardened rendering and plasteringmortar on substrates 12
- Determination of water-soluble chloride content of fresh mortar 13
- Determination of water absorption coefficient due to capillaryaction of hardened mortar 14
- Determination of water vapor permeability of hardened rendering and plastering mortars 14
- Determination of the compatibility of one-coat rendering mortarwith substrates 15
BS 4551: Methods of test for mortar 16
- Determination of consistence by dropping ball 16
- Determination of consistence retentivity and water retentivity 17
- Free water content 17
- Available lime content 17
- Other chemical tests 17
Glossary of Terms 19
Self-assessment Questions 20
Answers to Self-assessment Questions 21
Web sites and artwork:QPA Sites:QPA - MIA:Extras:MIA website update material:learning text:LT - Mortar Testing Ap#7E2.docPage 3 of 20Final Version
This learning text considers the topic of testing fresh and hardened mortar. The reasons fortesting are discussed, followed by a synopsis of the test methods. A glossary of terms is alsoincluded.
Two standards are applicable to the testing of mortar, namely:
BS EN 1015 - Methods of test for mortar for masonry (a multi part standard) BS 4551 - Methods of test for mortar.
Testing is generally undertaken for four principal reasons:
To evaluate conformity with a specification or Standard To control or monitor the consistency of a product or process To examine performance under project specific conditions To investigate problems and resolve disputes
There are four main forms of testing which can be undertaken:
i) Production Control Testing: Construction materials and component producers oftenundertake testing to monitor and control their production process. This should not beconfused with conformity evaluation, even though the same test methods may be used,as their purpose is entirely different.
ii) Performance Testing: Performance testing involves for example prism or cube testing,testing hardened mortar specimens to determine the water vapour permeability orconcrete pipes for leaks. Performance testing is becoming more important as newproduct standards are being written in terms of a performance requirement rather thanbeing based on a recipe.
iii) Compliance Testing: This involves testing materials or components against therequirements of the contract specification or Standard.
iv) Forensic Testing: This involves investigating problems in order to resolve disputese.g. chemical analysis of hardened mortar for cement or air content.
The results of production control and/or performance testing may be used for the evaluationof conformity.
The volume of standards and other regulatory documents that relate to the conduct of testingand calibration is increasing on a National, European and International scale. Within theUnited Kingdom, laboratories engaged in testing and calibration may seek accreditation fromThe United Kingdom Accreditation Service (UKAS). Accreditation may be sought for asingle test or for a wide range of tests.
Laboratories wishing to be accredited by UKAS are required to submit a quality manual toUKAS for approval. The quality manual has to be drafted to comply with the requirements ofBS EN ISO/IEC 17025:2000 - General requirements for the competence of testing andcalibration laboratories. Each test method requires individual accreditation.
Web sites and artwork:QPA Sites:QPA - MIA:Extras:MIA website update material:learning text:LT - Mortar Testing Ap#7E2.docPage 4 of 20Final Version
BS EN 1015 : Methods of Test For Mortar For Masonry
This is a multi part Standard, the individual parts that have been published are listed inTable 1. There are some gaps in the sequence of part numbers, this has occurred becausenumbers were allocated for the drafting of test methods that have subsequently beenwithdrawn from the standardization work programme.
Part 1 Determination of particle size distribution (by sieve analysis).Part 2 Bulk sampling of mortars and preparation of test mortars.Part 3 Determination of consistence of fresh mortar (by flow table).Part 4 Determination of consistence of fresh mortar (by plunger penetration).Part 6 Determination of bulk density of fresh mortar.Part 7 Determination of air content of fresh mortar.Part 9 Determination of workable life and correction time of fresh mortar.Part 10 Determination of dry bulk density of hardened mortar.Part 11 Determination of flexural and compressive strength of hardened mortar.Part 12 Determination of adhesive strength of hardened rendering and plastering mortars
on substrates.Part 17 Determination of water-soluble chloride content of fresh mortars.Part 18 Determination of water absorption coefficient due to capillary action of hardened
mortar.Part 19 Determination of water vapour permeability of hardened rendering and plastering
mortars.Part 21 Determination of the compatibility of one-coat rendering mortars with substrates.
Table 1 : BS EN 1015 - Methods of Test for Mortar for Masonry
Each of the individual parts of the Standard will be considered in turn.
i) There is a requirement in several parts of the Standard that ready-to-use mortars shallbe tested within their specified working life.
ii) Several parts of the Standard have a requirement that the minimum volume of thesample of fresh mortar shall be at least 1.5 litres or 1.5 times the volume (whichever isthe greater) needed to perform the test.
iii) Prior to testing samples of fresh mortar they should be gently stirred by hand for fiveto ten seconds with a palette knife.
iv) Where moulds/sample containers are filled with fresh mortar they should be filled tooverflowing and the excess struck off with a palette knife.
Web sites and artwork:QPA Sites:QPA - MIA:Extras:MIA website update material:learning text:LT - Mortar Testing Ap#7E2.docPage 5 of 20Final Version
v) Bulk samples may be reduced in size by the use of sample dividers or coning andquartering, the learning text on aggregates provides more detailed information on thissubject.
Determination of Particle Size Distribution (By Sieve Analysis):BS EN 1015-1
This part of the Standard prescribes the procedure for determining the particle sizedistribution of dry mixed or non hardened mortar or non hardened wet mixed mortar. The testis undertaken by placing individual sieves on top of each other to form what is called a nestof sieves (Figure 1). Table 2 lists the sieves that should be used:
Sieve Aperturesize - mm
Table 2 : Sieves required for mortar testing
Figure 1 : A nest of sieves
The test sample is placed in the top sieve of the nest and the sieves are agitated until materialceases to pass each of the sieves, the mass of material retained on each sieve is thendetermined. The Standard describes two alternative methods of undertaking sieve analysis,wet sieving and dry sieving. Where wet sieving is undertaken water is poured over the testsample in a container. This is then mixed and poured into the top sieve of the nest, a cover isthen placed over the top sieve and the nest agitated, each sieve and its residue is gentlywashed with a jet of water to ensure no undersize material remains on the sieve. Whenmaterial ceases to pass each sieve the material is removed and placed on individual trays anddried in an oven at 105 + 5oC until a constant mass is obtained.
Where dry sieving is to be undertaken the material is dried in an oven at 105 + 5oC until a
Web sites and artwork:QPA Sites:QPA - MIA:Extras:MIA website update material:learning text:LT - Mortar Testing Ap#7E2.docPage 6 of 20Final Version
constant mass is obtained, prior to undertaking the sieve analysis. The Standard prescribesthat mortars containing lightweight material shall only be tested by the dry sieving method.Bulk sampling of mortars and preparation of test mortars : BS EN 1015-2
The sampling of any material is very important, if a sample is not representative of thematerial the test results will be invalid. The taking of samples may involve sampling frommoving conveyors, trucks or delivery vehicles. It is essential that all health and safetyrequirements be complied with to minimize the risk of accidents. This includes wearing theappropriate personal protective equipment.
i) Sampling from mixers
A minimum of three increments is taken by passing the sample receptacle across thestream of mortar being discharged from the mixer.
ii) Sampling from conveyors
The sample is taken at the discharge point of the conveyor by passing the samplereceptacle across the stream of mortar at the discharge point. Where it is not possibleto sample the discharge stream in one operation take a number of increments. Analternative method of sampling is to stop the conveyor, isolate the plant equipmentand use a scoop to sample the full width of the conveyor belt. Where sampleincrements are taken, not less than three increments should be taken.
iii) Sampling from hoppers
Where possible hoppers are sampled when they are being filled or during discharge,this is especially important with large hoppers, if this is not possible take a minimumof three increments from at least 100 mm below the surface. It is very important forsafety reasons that the person taking the sample never enters the hopper.
iv) Sampling from delivery vehicles
Samples are where possible taken when the vehicle is being filled, if this is notpossible and samples have to be taken from a full vehicle take the sample in the samemanner as used for sampling from hoppers.
Sampling may result in a number of increments being taken, these are combined andthoroughly mixed on an impervious surface to form a bulk sample. The bulk samples may bereduced in size to produce a test sample by taking increments at random places from themixed material and recombining these.
The Standard lists the information that must be recorded to produce a sampling certificate.This part of the Standard also prescribes how dry mortars should be mixed to prepare wet testsamples.
Web sites and artwork:QPA Sites:QPA - MIA:Extras:MIA website update material:learning text:LT - Mortar Testing Ap#7E2.docPage 7 of 20Final Version
Determination of Consistence of Fresh Mortar (by flow table):BS EN 1015-3
The flow value is determined by measuring the mean diameter of a test sample. The bulksample of fresh mortar is reduced to a minimum sample size of 1.5 litres. Where it is desiredto measure the flow of dry mortars these should be mixed with water in accordance with therequirements of BS EN 1015-2.The test procedure involves placing the mould (60 mm in height, internal diameter: base 100mm - top 70 mm) in the center of the flow table and filling it in two layers each layer beingtamped ten times with the tamper. It is important that the mould is held firmly in place duringthis operation. The excess mortar is removed from the top of the mould with the palette knifeand the area around the base of the mould cleaned with a cloth. A period of approximately 15seconds is allowed to elapse and the mould is then removed, the table is jolted 15 times at arate of one jolt per second. The diameter of the spread mortar is measured in two directions atright angles to each other using calipers, both results are reported.
Determination of Consistence of Fresh Mortar (by plunger penetration):BS EN 1015-4
This part of the Standard lists a second method of measuring consistence, for an individualmortar it is normally possible to derive a correlation with the flow table method. The principleof this method is that a plunger rod having a mass of 90 grams is allowed to fall from a heightof 100 mm above the mortar. A sample of fresh mortar is placed in a cylindrical vessel in twolayers, each layers being compacted with 10 strokes of the tamper (identical specification tothe tamper used for the flow table test). The cylindrical vessel is placed under the plungerstand and the plunger allowed to fall from a height of 100 mm above the surface of themortar, the depth of penetration is read from a scale on the plunger and recorded to thenearest millimeter.
Determination of Bulk Density of Fresh Mortar : BS EN 1015-6
The bulk density of mortar is determined by calculating the mass of mortar contained in aknown volume. A sample of fresh mortar with a minimum volume of 3 litres (or at least 1.5times the volume need to perform the test). Three different methods of filling and compactingthe mortar within the calibrated container which should have a volume of approximately 1litre are given are in the Standard, (the container used for determining the air content of freshmortar is suitable). The method to be used depends upon the consistence of the fresh mortaras determined by the flow table test
i) Flow value less than 140 mm (stiff mortar) - Vibration method
The calibrated container is filled with mortar using a scoop until it is overflowing it isthen placed on a vibrating table and vibration continued until no further settlement ofthe material is observed, extra material is added if necessary. The container is thenweighed to an accuracy of 1 gram.
ii) Flow value between 140 mm and 200 mm (Plastic mortar) - Shock method
The calibrated container is filled to approximately half its height with mortar using ascoop, the container is then tilted about 30 mm on alternate sides and allowed to fall
Web sites and artwork:QPA Sites:QPA - MIA:Extras:MIA website update material:learning text:LT - Mortar Testing Ap#7E2.docPage 8 of 20Final Version
ten times on to a solid base. Where the mortar contains an air entraining admixture thenumber of shocks is reduced to five. The container is then filled to overflowing andthe shock compaction repeated. The container is then weighed to an accuracy of1 gram.
iii) Flow value greater than 200 mm (Soft mortar)
The calibrated container is filled with mortar using a scoop until it is overflowing, theedges of the container are wiped clean with a damp cloth and the container weighed toan accuracy of 1 gram.
The bulk density (m in kg/m3) is calculated by use of the formula:m = (m2-m1)/Vv
m1 = mass of empty containerm2 = mass of container plus mortarVv = volume of container
Determination of air content of fresh mortar : BS EN 1015-7
Two methods are prescribed for measuring the air content of fresh mortar, the pressure andthe alcohol method. The pressure method is applicable for mortars with an air content lessthan 20%, the alcohol method is applicable to mortars with an air content greater than 20%.
i) Pressure method
The equipment consists of a sample container and a cover assembly, the container hasan approximate volume of 1 litre, (the equipment is shown in Figure 2) a tamper(identical specification to the tamper used for the flow table test, BS EN 1015-2) and apalette knife are also required.
Figure 2 : A pressure type air meter
The sample container is filled in four approximately equal layers, each layer iscompacted with ten strokes of the tamper, the palette knife is used to remove any
Web sites and artwork:QPA Sites:QPA - MIA:Extras:MIA website update material:learning text:LT - Mortar Testing Ap#7E2.docPage 9 of 20Final Version
excess mortar. The container is cleaned with a damp cloth, (the rim of the containershould be free of any adhering mortar otherwise a watertight seal may not beachieved) and the cover assembly clamped in position and the main air valve closed.Water is introduced through valve A (used to fill the container with water) until all theair is expelled through valve B (this allows the escape of air from the container). Air ispumped into the air chamber until a stabilized condition is reached, this is equal to thelevel determined during the calibration procedure. Valves A and B are closed and thevalve between the air chamber and the sample container is opened. When equilibriumis reached the air content is read from the pressure gauge. The actual air content isdetermined from the calibration curve and recorded to the nearest 0.1%.The calibration procedure involves obtaining a correlation between pressure and aircontents over the range 5-25%.
It should be noted that Annex A of BS EN 1015-7 contains a schematic diagram of theapparatus.
ii) Alcohol method
This test method involves filling a 500 ml graduated measuring cylinder withapproximately 200 ml of fresh mortar, the measuring cylinder is tapped to level themortar and the volume recorded to the nearest ml (Vm1). A mixture of 60% ethylalcohol and 40% water is added until the 500 ml mark is reached, a rubber bung isinserted in the top of the cylinder and the cylinder inverted twenty times. The mixtureis allowed to settle for five minutes and the level of the surface (Vmf) is then recordedto the nearest ml.
The air content is calculated by use of the formula:
L = (500-Vmf ) Vm1
and reported to the nearest 0.1%.
Both methods of determining the air content require that two individual tests are undertakenand the mean value reported. The individual results are required to be within 10% of the meanvalue reported otherwise the test procedure has to be repeated. The Standard also requires thatthe flow value be reported.
Determination of Workable Life and Correction Time of Fresh Mortar:BS EN 1015-9
This part of the Standard contains three test methods:
Method A- Workable life of general purpose mortar Method B- Workable life of thin layer mortar Method C- Correction time of thin layer mortar.
The Standard requires that the flow value of the mortar to be tested shall be determined.
i) Method A - Workable life of general purpose mortar
Web sites and artwork:QPA Sites:QPA - MIA:Extras:MIA website update material:learning text:LT - Mortar Testing Ap#7E2.docPage 10 of 20Final Version
The workable life of the fresh mortar is defined as the time measured in minutes atwhich the mortar exhibits a defined limit of resistance to the penetration of a standardrod forced into it. The test procedure involves filling a number of moulds (internaldiameter 75 mm and 50 to 100 mm high) with fresh mortar and measuring thepenetrative force.
The equipment required is a penetration rod with a diameter of 5 mm and anapproximate length of 65 mm, the lower 25 mm of the rod should have a diameter of6.175 mm and the end face of the rod should be flat. A brass washer of approximately20 mm diameter and an internal diameter such that the washer is held at the point ofthe change in diameter of the rod. The penetration rod is held in a drill stand thatallows the rod to be lowered over a minimum distance of 40 mm.
The moulds are filled in ten increments and each mould tapped four times on a solidbase after the addition of each increment. The moulds are stored at an air temperatureof 20o C + 2o C and at a relative humidity of 95%.
The moulds are placed on a weighing scale (minimum capacity 15 kg and maximumgraduations 100 g) situated under the penetration rod. The scale reading is noted (R1)and the penetration rod slowly lowered into the fresh mortar, (care should be takenthat the point of contact is at least 20 mm from the mould edge or from a previouspoint of contact with the fresh mortar. The reading on the scale is noted (R2), theincrease in mass (R1- R2) divided by three should is reported as the resistance topenetration.
The penetration resistance of non-retarded mortars is measured at intervals of fifteenminutes commencing thirty minutes before the expiry of the declared workable life.Measurements are continued until the prescribed limit of resistance is reached. Forretarded mortars the penetration is measured at intervals until it starts to increase andmeasurements continued until the prescribed limit of resistance is reached.
The time in minutes reported to the nearest minute to give a resistance of penetrationof 0.5 N/mm2 is reported as the workable life. (It will normally be necessary todetermine this value by interpolation).
ii) Method B - Workable life of thin-layer mortar
The workable life is measured by the time taken in minutes for the flow value to differby more than 30 mm from the flow value measured 10 minutes after the mortar ismixed. The fresh mortar is maintained at an air temperature of 20oC + 2oC. The testprocedure requires that the flow value is determined at intervals of 15 minutes and thepoint at which a difference in flow of 30 mm occurs is determined by interpolation.
iii) Method C - Correction time of thin-layer mortar
The correction time of thin-layer mortar is defined as the time in minutes at which50% of the contact surface of a cube placed on a layer of mortar applied on thespecified masonry substrate and then removed is covered with adhering mortar.
Web sites and artwork:QPA Sites:QPA - MIA:Extras:MIA website update material:learning text:LT - Mortar Testing Ap#7E2.docPage 11 of 20Final Version
The test procedure involves cutting cubes with dimensions 50 mm x 50 mm x 50 mmfrom the specified masonry unit. Prior to performing the test the cubes and masonryunits are dried. The drying temperature depends on the composition of the masonryunits (Table 1 in BS EN 1015-9 lists the requirements). A cycle of drying andweighing is maintained until two consecutive readings taken at an interval two hoursapart do not differ by more than 0.2% by mass.
The masonry units are then stored at a temperature of 20oC + 2oC and at a relativehumidity of 65% + 5% for two days, testing is then carried out under the sameconditions. Mortar is applied to the masonry units with a trowel and then swept off,following this a layer of mortar 2 - 3 mm thick is then applied. A cube is then broughtinto contact with the mortar and maintained in position for thirty seconds, a load (theactual load depends on the density of the mortar unit) is maintained on the cube duringthis period. The cube is removed and the area covered with mortar determined. Thisprocedure is repeated at intervals of one minute until 50% of the cube contact area iscovered with adhering mortar.
Determination of Dry Bulk Density of Hardened Mortar : BS EN 1015-10
A sample of fresh mortar of minimum volume 50 times greater than the maximum aggregatesize (or 1.5 times the quantity needed to perform the test) whichever is the greater is required.Three test samples of regular shape are prepared from the fresh mortar to be tested and curedin accordance with BS EN 1015-11. The hardened test samples are dried to a constant mass ata temperature of 70oC (where organic material is incorporated a maximum temperature of65oC is used), the dry mass is recorded to the nearest 0.1% (mdry).
The test specimens are immersed in water (temperature 20oC + 2oC), the mass is noted after aperiod of immersion and the process repeated until the saturated mass does not differ by morethan 0.2%. The saturated mass is recorded to the nearest 0.1% (msat). The volume of the testspecimens is now determined by weighing the test specimens in water (using a stirrupattachment to the balance), the mass of the immersed test specimens is recorded to the nearest0.1% (mi).
The volume is calculated by use of the formula:
Vs = (msat - mi)/Density of water kg/m3
The bulk dry density of each test specimen is calculated from the volume:
Dry density (mdry)Volume
The mean dry density of the three test samples is required to be recorded to the nearest10 kg/m3
Determination of Flexural and Compressive Strength of Hardened Mortar:BS EN 1015-11
The flexural strength of a hardened mortar is determined by three point loading of a prismspecimen, subsequent to the failure and breakage of this specimen the compressive strength isdetermined on each half of the prism. Prism mould compartments are required to be 160 mmx 40 mm x 40 mm (each mould assembly produces three prism specimens), prior to use they
Web sites and artwork:QPA Sites:QPA - MIA:Extras:MIA website update material:learning text:LT - Mortar Testing Ap#7E2.docPage 12 of 20Final Version
are lubricated with a thin layer of mineral oil. Depending on the type of binder differentprocedures are applicable for the manufacture of the prisms.
i) Mortars produced from hydraulic binders and air-lime binders where the mass of air-lime is not greater than 50% of the total binder content:
The mould is filled in two layers each layer being compacted with twenty fivestrokes of the tamper. (Tamper: a rigid non-absorptive rod, with a square cross sectionof 12 x 12 mm and a mass of 50 grams).
ii) Mortars produced from air-lime and air-lime cement binders with a cement mass lessthan 50% of the total binder content:
The mould is placed on a glass plate, on which two layers of white cotton gauze havebeen placed, the mould is filled and compacted as described in i). Two layers of cottongauze are placed on top of the compacted prisms followed by six layers of absorbentfilter paper. A glass plate is placed on top of the mould and the whole assemblyinverted, the glass plate is then carefully removed and six layers of filter paper placedon top of the gauze and the glass plate replaced. The wholly assembly is then re-inverted and an approximate mass of 5 kg placed on top of the glass plate and theassembly left undisturbed for a period of three hours. At the end of this period the topglass plate is removed and the filter paper and gauze discarded. The glass plate is thenreplaced, the assembly inverted, the glass plate is removed and the gauze and filterpaper discarded. The test specimens are then cured.
Initial curing may be carried out either in a polythene bag or in a curing chamber, part of theinitial curing period is undertaken with the test specimen removed from the mould.
The main curing period is undertaken in a curing chamber, Table 1 in BS EN 1015-11 liststhe time periods for the different stages of curing which are dependent on the type of binderused.
The determination of flexural strength is undertaken when the test specimens are twenty-eightdays old, the testing machine is required to have two supporting rollers and a third roller (theloading roller, located above the test specimen and midway between the supporting rollers).The prism is placed so that one of its faces, which has been cast against the steel mould, is incontact with the supporting rollers. The load is applied to the test specimens at a rate thatproduces failure in a time period of thirty to ninety seconds. The flexural strength (f) iscalculated from the equation:
f = 1.5 Fl bd2
Where b and d are the internal dimensions of the prism mould, l is the distance between thesupporting rollers. The result is recorded to the nearest 0.05 N/mm2 and the average of the setof results reported to the nearest 0.1 N/mm2.
The compressive strength is determined on the broken halves of the prism by using acompression jig in a testing machine care being taken that the load is applied to a face castagainst the steel face of the mould. The load is applied to the test specimens at a rate that
Web sites and artwork:QPA Sites:QPA - MIA:Extras:MIA website update material:learning text:LT - Mortar Testing Ap#7E2.docPage 13 of 20Final Version
produces failure in a time period of thirty to ninety seconds. The compressive strength isrecorded to the nearest 0.05 N/mm2 and the mean result reported to the nearest 0.1 N/mm2.
Determination of Adhesive Strength of Hardened Rendering and PlasteringMortar on Substrates: BS EN 1015-12
This test method involves determining the maximum tensile stress applied by a direct load atright angles to the surface of the rendering. Where the rendering mortar is designed for usewith a particular type of masonry, it is tested with samples of the appropriate masonry. If nospecific background (substrate) is specified, concrete panels with minimum dimensions 550mm x 150 mm x 50 mm (thickness) are used. The panels are prepared from concrete with awater cement ratio of 0.55 and graded aggregates with a maximum particle size of one thirdof the panel thickness. The concrete panels are wood floated to provide a suitable surface andare required to be at least twenty eight days old when testing is undertaken.
The fresh mortar that is to be tested is applied to the relevant substrate to achieve a thicknessof 10 mm + 1 mm. Two options exist for sampling the test specimen. Firstly, a sample may beobtained after initial setting of the mortar by pressing the sharp edge of a lightly oiledtruncated conical metal ring (internal diameter 50 mm and 25 mm high) into the mortar untilthe substrate is reached. Secondly, a sample may be obtained where it is hardened by using acore drill with a similar internal diameter and drilling into the mortar and substrate. (Drillingshould be to a depth of 2 mm into the substrate).
The test specimens are stored in an airtight polythene bag at a temperature of 20o C + 2o Cfor seven days and then for twenty one days in a humidity chamber at a similar temperatureand a humidity of 65% + 5%. The test specimens are tested immediately on removal from thehumidity chamber.
The pull head is glued (the adhesive should be epoxy resin or methyl methylmethacrylateresin) to the mortar surface care being taken to prevent the adhesive bridging the cut area. Thetesting machine is connected to the pull head and a perpendicular tensile load applied, thefailure load is recorded, the rate of application of the load depending on the anticipatedadhesive strength, Table 2 of BS EN 1015-12 lists the requirements. Five test specimens areused, the individual adhesive strengths are recorded to the nearest 0.05 N/mm2 and the meanvalue to the nearest 0.1 N/mm2.
The Standard incorporates three figures illustrating the type of fracture pattern that can occur:
Fracture at the interface between the mortar and substrate. Fracture within the mortar. Fracture in the substrate material.
Determination of Water-Soluble Chloride Content of Fresh Mortar:BS EN 1015-17
This is the only chemical test method within the BS EN 1015 series of Standards. The testmethod is based on the formation of a soluble coloured compound, this analytical technique issometimes referred to as the Volhard method, named after the chemist who developed it in1878. The principle of this analytical technique is that the chloride solution is treated with an
Web sites and artwork:QPA Sites:QPA - MIA:Extras:MIA website update material:learning text:LT - Mortar Testing Ap#7E2.docPage 14 of 20Final Version
excess of silver nitrate and the residual silver nitrate determined by titration with ammoniumthiocyanate. The chloride ion present in the test sample reacts with the silver nitrate to formsilver chloride, the titration with ammonium thiocyanate allows the analyst to determine howmuch silver nitrate has reacted.
The sample has to be in a dry state, where a sample of fresh mortar has been taken this isdried in an oven at a temperature of 105oC + 5oC, the sample is then ground to pass through a0.125 mm test sieve. The water soluble chloride is extracted by placing a 10 gram sample in apolythene bottle and adding 100 ml of distilled or deionized water. The sample is shaken forapproximately 60 minutes and then allowed to stand for a minimum period of 15 hours and amaximum period of 24 hours.
The sample is then filtered, 20 ml of dilute nitric acid is added to the filtrate and the solutionis boiled. To the boiling solution 5 ml of silver nitrate solution is added and after a further2 minutes boiling the solution is cooled to below 25oC. A chemical indicator is then added tothe solution and ammonium thiocyanate is added drop wise from a burette until a permanentreddish brown colour is obtained, the quantity added is recorded. The volume of silver nitratethat has reacted is calculated and by the use of a chemical formula the chloride content of thesample is determined. The Standard gives details of the concentration (molarity) of thechemical solutions that should be used.
Determination of Water Absorption Coefficient Due to Capillary Action ofHardened Mortar: BS EN 1015-18
This test procedure is undertaken using mortar prism specimens that are dried to a constantmass, one face of the prism is immersed in water for a specified period of time and theincrease in mass is determined. A prism mould (see section on BS EN 1015-11) is lined atthe base with absorbent filter paper and filled with fresh mortar, the top surface is alsocovered with a layer of filter paper. The test specimens are then cured for an initial period,part of the initial curing period is undertaken with the specimen removed from the mould. Themain curing period is undertaken in a curing chamber. Table 1 of BS EN 1015-18 lists thetime periods for the different stages of curing which are dependent on the type of binder used.
At the completion of the curing period of the test specimens the long faces are sealed withparaffin wax (or a synthetic reactive resin with a melting point above 60oC) and are thenbroken into half. The test specimens are then dried in an oven at 60oC + 5 oC until twosuccessive weighings undertaken twenty fours apart give a mass variation of less than 0.2% ofthe total mass.
The test specimens are placed broken end downwards on four support pads (these should haveas small an area as possible) in a tray (having a minimum depth of 20 mm). The testspecimens are immersed to a depth of 5-10 mm in water and the tray covered to minimizeevaporation. The time of immersion is noted
The procedure now varies, for renovation mortars a modified procedure is followed. The testspecimens (all mortars except renovation) are removed from the tray after ten minutes. Thesurface water is wiped off with a damp cloth and the mass determined, the test specimens arereplaced in the tank and the mass determined using the same procedure after ninety minutes.Where renovation mortars are being tested the test specimens are immersed for a twenty four
Web sites and artwork:QPA Sites:QPA - MIA:Extras:MIA website update material:learning text:LT - Mortar Testing Ap#7E2.docPage 15 of 20Final Version
hour period, on removal from the tray they are weighed, they are then split along the longdimension and the depth of water penetration measured to the nearest 1 mm.
The coefficient of water absorption is calculated using the appropriate formulae given in theStandard.
Determination of Water Vapour Permeability of Hardened Rendering andPlastering Mortars: BS EN 1015-19
The procedure for this test method involves the production of disc shaped specimens that arethen exposed to water vapour pressure, the rate of moisture transfer is determined by thechange in mass. The test specimens are produced by applying a layer of mortar (10-30 mmthick and slightly larger in diameter than the cups) to a substrate of aerated concrete (density550 kg/m3 + 50 kg/m3), prior to the application of the mortar place two layers of cotton gauzeon the substrate. Five test specimens are prepared for each hydroscopic range. The testspecimens are cured for a total period of twenty eight days, Table 1 of BS EN 1015-19 liststhe requirements for the initial curing period and the main curing period, the requirementsdepend upon the type of binder used.
At the end of the curing period the specimens are cut to the dimensions of the test cups (thetest cups should be made of corrosion resisting material and have an area of approximately0.02 m2). The test specimens are then placed in the test cups and the edges sealed with animpermeable sealant, which remains constant in mass under the test conditions. The cups aremanufactured so that the test specimen is held on a ledge below which the chemical solutionis placed there must be an air gap of 10 mm + 5 mm between the test specimen and thechemical solution (Figure 1 in the Standard provides an illustration). The test cups are placedin the curing chamber at a temperature of 20oC + 2oC and at a relative humidity of 50% + 5%.
The test cups are weighed at intervals and a graph drawn plotting time against mass, if threepoints can be placed on a straight line the quantity of water vapour passing through the testspecimen is taken to be constant. A formula is given in BS EN 1015-19 to calculate the watervapour permeability
Two hydroscopic ranges are tested. Samples are prepared in exactly the same way butdifferent chemical solutions are used. A saturated solution of potassium nitrate provides arelative humidity of 93.2% and a saturated solution of lithium chloride provides a relativehumidity of 12.4% at a temperature of 20oC + 2oC.
Determination of The Compatibility of One-Coat Rendering Mortar withSubstrates: BS EN 1015-21
This test method evaluates the compatibility of one coat rendering mortar with a givensubstrate, the samples are brought to a standard condition and then subjected to two tests,which evaluate the water permeability and the adhesion strength. The test specimen isprepared on either a concrete substrate (minimum dimensions 300 mm x 300 mm x 40 mm)or on a masonry substrate (minimum dimensions 400 mm x 400 mm made from at least onewhole and two half masonry units). The fresh mortar is applied to the vertical substrate, twotest panels are produced one with a mortar thickness of 10 mm and the other 20 mm. The testspecimens are cured for a minimum of twenty eight days at a temperature of 20oC + 2oC and a
Web sites and artwork:QPA Sites:QPA - MIA:Extras:MIA website update material:learning text:LT - Mortar Testing Ap#7E2.docPage 16 of 20Final Version
relative humidity of 65% + 5%. The test specimens are then subjected to a two stageconditioning process.
On completion of curing the test specimens are firstly subjected to four heating and freezingcycles. The test specimens are heated by an infrared lamp to a temperature of 60oC + 2oC fora period of eight hours, they are then placed in the standardized curing conditions for thirtyminutes. Following this the samples are placed in a deep freeze cabinet (temperature 15oC +1oC) for fifteen hours, the test specimens are then placed in the standardized curing conditionsfor thirty minutes. The cycle is repeated four times, after completion of the fourth cycle thetest specimens are placed in the standardized curing conditions for a minimum of forty eighthours.
The second stage of the conditioning process is then undertaken. The test specimens arepartially immersed in water (temperature 20oC + 2oC), with the rendered sides in the water toan approximate depth of 5 mm for a period of eight hours. They are then placed in thestandardized conditions used for curing for thirty minutes. Following this the samples areplaced in a deep freeze cabinet (temperature 15oC + 1oC) for fifteen hours, the testspecimens are then placed in the standardized curing conditions for thirty minutes.
During each stage of the conditioning cycle the test specimens are examined for any signs ofdamage and a record made of any deterioration.
The test specimens are then tested for water permeability, prior to undertaking this test thetest specimens are maintained in the standard curing conditions for forty eight hours (Figure 1of BS EN 1015-21 illustrates the test apparatus). A metal cone with a base diameter of 200mm and a height of 100 mm is required to be bonded to the rendered surface of the testspecimen using a water resistant sealant. A head of water of 100 mm above the surface ismaintained for a period of forty eight hours, the quantity of water required to maintain thishead is recorded to the nearest 1 ml. The water permeability is calculated as the quantity ofwater required to maintain a constant level divided by 100, ml/cm2, the result is reported asml/(cm2.48 h) to the nearest 0.1 ml/cm2.48 h.
Following completion of the water permeability test the test specimens are placed in thestandard curing conditions for a minimum of four days, the adhesive strength is thendetermined and reported in accordance with the requirements of BS EN 1015-12.
BS 4551 : Methods of Test for Mortar
Historically this Standard has been published in two parts, Part 1 covered the physical testsand Part 2 the chemical tests. This Standard has now been revised and published as a singledocument. The majority of the physical tests for mortar for masonry are covered by BS EN1015, the two exceptions are:
Determination of consistence by dropping ball Determination of consistence retentivity and water retentivity.
The Standard also covers the chemical tests for mortar, which have not yet been addressedwithin the European standardization programme.
Web sites and artwork:QPA Sites:QPA - MIA:Extras:MIA website update material:learning text:LT - Mortar Testing Ap#7E2.docPage 17 of 20Final Version
Determination of Consistence by Dropping Ball
This test method determines the penetration of a ball made of methyl methylmethacrylate intoa test sample of fresh mortar when dropped from a prescribed height. A mould made of rigidmaterial (internal diameter 100 mm, height 25 mm) is filled with fresh mortar inapproximately ten increments pushing the mortar into the mould with the palette knife, theexcess mortar is struck off with a palette knife. The ball is held in a mechanism and droppedfrom a height 250 mm above the test specimen, the ball mechanism is positioned so that theball falls in the approximate centre of the fresh mortar (+ 12 mm). The penetration of the ballis measured to the nearest 0.1 mm using the measuring device. Three separate determinationsof penetration are made and the mean value reported.
Web sites and artwork:QPA Sites:QPA - MIA:Extras:MIA website update material:learning text:LT - Mortar Testing Ap#7E2.docPage 18 of 20Final Version
Determination of Consistence Retentivity and Water Retentivity
This test procedure determines the change in the level of consistence when the mortar issubjected to suction and the loss of water from the fresh mortar. The mould (as described inthe previous section) is weighed, eight discs of filter paper are also weighed. The consistenceby dropping ball is then determined, the depression left by the penetration is filled and thefresh mortar struck off with the palette knife. The mould and its contents are then weighed.Two pieces of cotton gauze and the eight discs of filter paper are placed on top of the mortarand a non porous plate is placed on top of these together with a 2 kg weight. A period of twominutes is allowed to elapse, the weight and plate removed, the cotton gauze discarded andthe filter papers weighed to the nearest 0.05 grams.
The mass of water remaining in the mould (i.e. the mass of water originally in the mortarminus the water absorbed by the filter paper) is expressed as a percentage of the originalwater content of the fresh mortar and reported as the water retentivity. The original watercontent may be determined as described in the next section.
Any fall in the level of the mortar in the mould is measured and recorded, the penetrationdetermined by the dropping ball should again be undertaken. A correction is made for anymeasured fall in level (subtract the fall in level from the penetration depth). The correctedpenetration is reported as a percentage of the penetration before suction as the consistenceretentivity. The determination is repeated and the mean water retentivity reported to thenearest 1%, the mean consistence retentivity is reported to the nearest 5%.
Free Water Content
The free water content is determined by weighing a 10 + 1 gram sample into a tared dish anddrying in the oven at 105oC + 5 oC until a constant mass is obtained. The free water content isreported as the loss in mass expressed as a percentage of the original wet mass.
Available Lime Content
A 5 + 0.05 gram sample is weighed into a 250 ml conical flask containing 30 ml of distilledwater, the flask is stoppered and swirled, the stopper is loosened and the contents heated toboiling and the flask then allowed to simmer for two minutes. The flask is then removed fromthe heat source, 150 ml of water and 15 grams of granulated sugar added. The flask isstoppered and shaken vigorously and allowed to stand for a minimum period of thirty minutesand a maximum period of one hour.A chemical indicator is then added and the solution titrated with hydrochloric acid until thecolouration disappears. The Standard gives details of the concentration of the acid solutionand the formula for calculating the available lime content.
Other Chemical Tests
The Standard also prescribes how a range of more complex chemical tests are undertaken: insoluble residue, soluble silica, calcium oxide, sulfur trioxide,
Web sites and artwork:QPA Sites:QPA - MIA:Extras:MIA website update material:learning text:LT - Mortar Testing Ap#7E2.docPage 19 of 20Final Version
total iron, aluminium oxide, magnesium oxide.
To undertake these tests accurately and safely specialist training in analytical techniques isrequired and therefore they are not discussed further in this learning text. Chemical analysisrequires the use of very small sample sizes and even greater care must be taken whensampling mortars for these techniques.
Glossary of terms
Bulk sample - A sample comprising a mixture of all the individual increments taken.
Burette- - A graduated glass tube with a tap for measuring the volume of liquid run out from it.
Chemical Indicator - A substance that by a sharp colour change indicates the completion ofa chemical reaction.
Consistence - The fluidity of a fresh mortar.
Density - The mass per unit volume of a substance.
Bulk Density - The density of a porous or granular material calculated per unitvolume of the substance including pores or spaces, it is less than thetrue or absolute density of the material.
Filtrate - A substance that has been filtered and contains no suspended matter.
Hydgroscopic - A material that has a tendency to absorb moisture.
Increment - Quantity of material taken in a single operation of the samplingequipment used.
Molarity - A method of expressing the strength of a chemical solution. .Relative Humidity - Humidity is the amount of moisture in the air, there are various
methods of measuring and reporting it. The most common format isrelative humidity- this is the amount of water vapour present in the airexpressed as the amount of water vapour that the air can hold at thattemperature. Because temperature greatly affects water vapour, airthat has only a 30% relative humidity at 30oC has 100% relativehumidity at 10 oC. At 100% relative humidity dew would form on theground.
Renovation Mortar - A designed rendering/plastering mortar for use on moist masonrywalls containing soluble salts. These mortars have a high porosity andvapour permeability and reduce capillary action.
Saturated Solution - A solution where no material can be dissolved at that temperature.
Web sites and artwork:QPA Sites:QPA - MIA:Extras:MIA website update material:learning text:LT - Mortar Testing Ap#7E2.docPage 20 of 20Final Version
Thin-layer Mortar - A designed masonry mortar for use in joints between 1 and 3 mmthick, with a maximum aggregate size less than or equal to 2 mm.
Titration - The addition of a measured amount of one reagent to a definiteamount of another reagent until the reaction between them iscomplete. (until the second reagent is completely used up).
1 What two Standards are concerned with mortar testing?
2 What is the minimum number of sample increments that should be taken?
3 What are the three methods of determining consistence?
4 How is the bulk density of fresh mortar calculated?
5 Which method of measuring air content should be used for a mortar with an aircontent greater than 20%?
6 Which are the two main chemical reagents used in the determination of watersoluble chloride?
7 How is the correction time of thin-layer mortar defined?
8 What test method is used to determine the workable life of thin-layer mortar?
9 What type of test specimens are used to determine the compressive strength ofmortar?
10 How is relative humidity defined?
Web sites and artwork:QPA Sites:QPA - MIA:Extras:MIA website update material:learning text:LT - Mortar Testing Ap#7E2.docPage 21 of 20Final Version
Answers to Self-Assessment Questions
1 BS EN 1015 - Methods of test for mortar for masonry.BS 4551 - Methods of test for mortar.
3 Flow tablePlunger penetrationDropping ball.
4 The bulk density is calculated by dividing the mass of material by the volume itoccupies.
5 The alcohol method should be used for measuring air contents greater than 20%.
6 Silver nitrate and Ammonium thiocyanate.
7 The correction time of thin-layer mortar is defined as the time in minutes at which50% of the contact surface of a cube placed on a layer of mortar applied on thespecified masonry substrate and then removed is covered with adhering mortar.
8 The flow table test.
9 The two broken parts of a prism.
10 Relative humidity is expressed as a percentage, 100% relative humidity means that theair is saturated or completely full of water. The higher the temperature the greater thequantity of water vapour the air can hold.
Click here to load reader